Download presentation

Presentation is loading. Please wait.

Published byJailyn Alder Modified over 2 years ago

1
Objective Linear Ferro- magnets Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry 1 Anisotropic Elasticity 27-750 Texture, Microstructure & Anisotropy A.D. Rollett Last revised: 7 th Feb. 14

2
Objective Linear Ferro- magnets Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry 2Bibliography R.E. Newnham, Properties of Materials: Anisotropy, Symmetry, Structure, Oxford University Press, 2004, 620.112 N55P. Nye, J. F. (1957). Physical Properties of Crystals. Oxford, Clarendon Press. Kocks, U. F., C. Tomé and R. Wenk (1998). Texture and Anisotropy, Cambridge University Press, Cambridge, UK. Chapter 7. T. Courtney, Mechanical Behavior of Materials, McGraw-Hill, 0-07-013265-8, 620.11292 C86M. Reid, C. N. (1973). Deformation Geometry for Materials Scientists. Oxford, UK, Pergamon. Newey, C. and G. Weaver (1991). Materials Principles and Practice. Oxford, England, Butterworth-Heinemann.

3
Objective Linear Ferro- magnets Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry 3Notation F Stimulus (field) R Response P Property j electric current E electric field D electric polarization Strain Strain Stress (or conductivity) Stress (or conductivity) Resistivity Resistivity d piezoelectric tensor C elastic stiffness S elastic compliance a transformation matrix W work done (energy) dW work increment I identity matrix O symmetry operator (matrix) Y Youngs modulus Kronecker delta Kronecker delta e axis (unit) vector T tensor direction cosine direction cosine

4
Objective Linear Ferro- magnets Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry 4Objective The objective of this lecture is to provide a mathematical framework for the description of properties, especially when they vary with direction. A basic property that occurs in almost applications is elasticity. Although elastic response is linear for all practical purposes, it is often anisotropic (composites, textured polycrystals etc.). Why do we care about elastic anisotropy? In composites, especially fibre composites, it is easy to design in substantial anisotropy by varying the lay-up of the fibres. See, for example: http://www.jwave.vt.edu/crcd/kriz/lectures/Geom_3.html http://www.jwave.vt.edu/crcd/kriz/lectures/Geom_3.html Geologists are very familiar with elastic anisotropy and exploit it for understanding seismic results.

5
Objective Linear Ferro- magnets Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry In Class Questions 1.Why is plastic yielding a non-linear property, in contrast to elastic deformation? 2.What is the definition of a tensor? 3.Why is stress is 2 nd -rank tensor? 4.Why is elastic stiffness a 4 th -rank tensor? 5.What is matrix notation (in the context of elasticity)? 6.What are the relationships between tensor and matrix coefficients for stress? Strain? Stiffness? Compliance? 7.Why do we need factors of 2 and 4 in some of these conversion factors? 8.How do we use crystal symmetry to decrease the number of coefficients needed to describe stiffness and compliance? 9.How many independent coefficients are needed for stiffness (and compliance) in cubic crystals? In isotropic materials? 10.How do we express the directional dependence of Youngs modulus? 11.What is Zeners anisotropy factor? 5

6
Objective Linear Ferro- magnets Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry 6 Anisotropy: Practical Applications The practical applications of anisotropy of composites, especially fiber-reinforced composites are numerous. The stiffness of fiber composites varies tremendously with direction. Torsional rigidity is very important in car bodies, boats, aeroplanes etc. Even in monolithic polymers (e.g. drawn polyethylene) there exists large anisotropy because of the alignment of the long-chain molecules.

7
Objective Linear Ferro- magnets Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry 7 Application example: quartz oscillators Piezoelectric quartz crystals are commonly used for frequency control in watches and clocks. Despite having small values of the piezoelectric coefficients, quartz has positive aspects of low losses and the availability of orientations with negligible temperature sensitivity. The property of piezoelectricity relates strain to electric field, or polarization to stress. ij = d ijk E k PZT, lead zirconium titanate PbZr 1-x Ti x O 3, is another commonly used piezoelectric material.

8
Objective Linear Ferro- magnets Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry Piezoelectric Devices 8 [Newnham] The property of piezoelectricity relates strain to electric field, or polarization to stress. ij = d ijk E k PZT, lead zirconium titanate PbZr 1-x Ti x O 3, is another commonly used piezoelectric material. Note: Newnham consistently uses vector-matrix notation, rather than tensor notation. We will explain how this works later on. Examinable

9
Objective Linear Ferro- magnets Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry Piezoelectric Crystals How is it that crystals can be piezoelectric? The answer is that the bonding must be ionic to some degree (i.e. there is a net charge on the different elements) and the arrangement of the atoms must be non-centrosymmetric. PZT is a standard piezoelectric material. It has Pb atoms at the cell corners ( a~4Å ), O on face centers, and a Ti or Zr atom near the body center. Below a certain temperature (Curie T), the cell transforms from cubic (high T) to tetragonal (low T). Applying stress distorts the cell, which changes the electric displacement in different ways (see figure). Although we can understand the effect at the single crystal level, real devices (e.g. sonar transducers) are polycrystalline. The operation is much complicated than discussed here, and involves poling to maximize the response, which in turns involves motion of domain walls. 9 [Newnham]

10
Objective Linear Ferro- magnets Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry 10 Mathematical Descriptions Mathematical descriptions of properties are available. Mathematics, or a type of mathematics provides a quantitative framework. It is always necessary, however, to make a correspondence between mathematical variables and physical quantities. In group theory one might say that there is a set of mathematical operations & parameters, and a set of physical quantities and processes: if the mathematics is a good description, then the two sets are isomorphous. This lecture makes extensive use of tensors. A tensor is a quantity that can be transformed from one set of axes to another via the tensor transformation rule (next slide).

11
Objective Linear Ferro- magnets Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry 11 Tensor: definition, contd. In order for a quantity to qualify as a tensor it has to obey the axis transformation rule, as discussed in the previous slides. The transformation rule defines relationships between transformed and untransformed tensors of various ranks. Vector: V i = a ij V j 2 nd rank T ij = a ik a jl T kl 3 rd rank T ijk = a il a jm a kn T lmn 4 th rank T ijkl = a im a jn a ko a lp T mnop This rule is a critical piece of information, which you must know how to use.

12
Objective Linear Ferro- magnets Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry 12 Non-Linear properties, example Another important example of non-linear anisotropic properties is plasticity, i.e. the irreversible deformation of solids. A typical description of the response at plastic yield (what happens when you load a material to its yield stress) is elastic-perfectly plastic. In other words, the material responds elastically until the yield stress is reached, at which point the stress remains constant (strain rate unlimited). A more realistic description is a power-law with a large exponent, n~50. The stress is scaled by the crss, and be expressed as either shear stress- shear strain rate [graph], or tensile stress-tensile strain [equation]. [Kocks]

13
Objective Linear Ferro- magnets Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry 13 Linear properties Certain properties, such as elasticity in most cases, are linear which means that we can simplify even further to obtain R = R 0 + PF or if R 0 = 0, R = PF. e.g. elasticity: = C In tension, C Youngs modulus, Y or E. stiffness

14
Objective Linear Ferro- magnets Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry 14Elasticity Elasticity: example of a property that requires tensors to describe it fully. Even in cubic metals, a crystal is quite anisotropic. The [111] in many cubic metals is stiffer than the [100] direction. Even in cubic materials, 3 numbers/coefficients/moduli are required to describe elastic properties; isotropic materials only require 2. Familiarity with Miller indices, suffix notation, Einstein convention, Kronecker delta, permutation tensor, and tensors is assumed.

15
Objective Linear Ferro- magnets Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry 15 Elastic Anisotropy: 1 First we restate the linear elastic relations for the properties Compliance, written S, and Stiffness, written C (admittedly not very logical choice of notation), which connect stress,, and strain,. We write it first in vector-tensor notation with : signifying inner product (i.e. add up terms that have a common suffix or index in them): = C: = S: In component form (with suffices), ij = C ijkl kl ij = S ijkl kl

16
Objective Linear Ferro- magnets Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry 16 Elastic Anisotropy: 2 The definitions of the stress and strain tensors mean that they are both symmetric (second rank) tensors. Therefore we can see that 23 = S 2311 11 32 = S 3211 11 = 23 which means that, S 2311 = S 3211 and in general, S ijkl = S jikl We will see later on that this reduces considerably the number of different coefficients needed.

17
Objective Linear Ferro- magnets Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry 17 Stiffness in sample coords. Consider how to express the elastic properties of a single crystal in the sample coordinates. In this case we need to rotate the (4 th rank) tensor stiffness from crystal coordinates to sample coordinates using the orientation (matrix), a : c ijkl ' = a im a jn a ko a lp c mnop Note how the transformation matrix appears four times because we are transforming a 4 th rank tensor! The axis transformation matrix, a, is sometimes also written as, also as the transpose of the orientation matrix g T.

18
Objective Linear Ferro- magnets Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry 18 Youngs modulus from compliance Young's modulus as a function of direction can be obtained from the compliance tensor as: E=1/s' 1111 Using compliances and a stress boundary condition (only 11 0) is most straightforward. To obtain s ' 1111, we simply apply the same transformation rule, s' ijkl = a im a jn a ko a lp s mnop

19
Objective Linear Ferro- magnets Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry 19 Voigt or matrix notation It is useful to re-express the three quantities involved in a simpler format. The stress and strain tensors are vectorized, i.e. converted into a 1x6 notation and the elastic tensors are reduced to 6x6 matrices.

20
Objective Linear Ferro- magnets Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry 20 matrix notation, contd. Similarly for strain: The particular definition of shear strain used in the reduced notation happens to correspond to that used in mechanical engineering such that 4 is the change in angle between direction 2 and direction 3 due to deformation.

21
Objective Linear Ferro- magnets Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry 21 Work conjugacy, matrix inversion The more important consideration is that the reason for the factors of two is so that work conjugacy is maintained. dW = :d ij : d ij = k d k Also we can combine the expressions = C and = S to give: = CS, which shows: I = CS, or, C = S -1

22
Objective Linear Ferro- magnets Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry 22 Tensor conversions: stiffness Lastly we need a way to convert the tensor coefficients of stiffness and compliance to the matrix coefficients. For stiffness, it is very simple because one substitutes values according to the following table, such that matrix C 11 = tensor C 1111 for example.

23
Objective Linear Ferro- magnets Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry 23 Stiffness Matrix

24
Objective Linear Ferro- magnets Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry 24 Tensor conversions: compliance For compliance some factors of two are required and so the rule becomes:

25
Objective Linear Ferro- magnets Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry 25 Relationships between coefficients: C in terms of S Some additional useful relations between coefficients for cubic materials are as follows. Symmetrical relationships exist for compliances in terms of stiffnesses (next slide). C 11 = (S 11 +S 12 )/{(S 11 -S 12 )(S 11 +2S 12 )} C 12 = -S 12 /{(S 11 -S 12 )(S 11 +2S 12 )} C 44 = 1/S 44.

26
Objective Linear Ferro- magnets Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry 26 S in terms of C The relationships for S in terms of C are symmetrical to those for stiffnesses in terms of compliances (a simple exercise in algebra). S 11 = (C 11 +C 12 )/{(C 11 -C 12 )(C 11 +2C 12 )} S 12 = -C 12 /{(C 11 -C 12 )(C 11 +2C 12 )} S 44 = 1/C 44.

27
Objective Linear Ferro- magnets Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry 27 Neumann's Principle A fundamental natural law: Neumann's Principle: the symmetry elements of any physical property of a crystal must include the symmetry elements of the point group of the crystal. The property may have additional symmetry elements to those of the crystal (point group) symmetry. There are 32 crystal classes for the point group symmetry. F.E. Neumann 1885.

28
Objective Linear Ferro- magnets Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry 28 Neumann, extended If a crystal has a defect structure such as a dislocation network that is arranged in a non-uniform way then the symmetry of certain properties may be reduced from the crystal symmetry. In principle, a finite elastic strain in one direction decreases the symmetry of a cubic crystal to tetragonal or less. Therefore the modified version of Neumann's Principle: the symmetry elements of any physical property of a crystal must include the symmetry elements that are common to the point group of the crystal and the defect structure contained within the crystal.

29
Objective Linear Ferro- magnets Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry 29 Effect of crystal symmetry Consider an active rotation of the crystal, where O is the symmetry operator. Since the crystal is indistinguishable (looks the same) after applying the symmetry operator, the result before, R (1), and the result after, R (2), must be identical: The two results are indistinguishable and therefore equal. It is essential, however, to express the property and the operator in the same (crystal) reference frame.

30
Objective Linear Ferro- magnets Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry 30 Symmetry, properties, contd. Expressed mathematically, we can rotate, e.g. a second rank property tensor thus: P' = OPO T = P, or, in coefficient notation, P ij = O ik O il P kl where O is a symmetry operator. Since the rotated (property) tensor, P, must be the same as the original tensor, P, then we can equate coefficients: P ij = P ij If we find, for example, that P 21 = -P 21,then the only value of P 21 that satisfies this equality is P 21 = 0. Remember that you must express the property with respect to a particular set of axes in order to use the coefficient form. In everything related to single crystals, always use the crystal axes as the reference frame!Remember that you must express the property with respect to a particular set of axes in order to use the coefficient form. In everything related to single crystals, always use the crystal axes as the reference frame! Homework question: based on cubic crystal symmetry, work out why a second rank tensor property can only have one independent coefficient.

31
Objective Linear Ferro- magnets Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry 31 Effect of symmetry on stiffness matrix Why do we need to look at the effect of symmetry? For a cubic material, only 3 independent coefficients are needed as opposed to the 81 coefficients in a 4th rank tensor. The reason for this is the symmetry of the material. What does symmetry mean? Fundamentally, if you pick up a crystal, rotate [mirror] it and put it back down, then a symmetry operation [rotation, mirror] is such that you cannot tell that anything happened. From a mathematical point of view, this means that the property (its coefficients) does not change. For example, if the symmetry operator changes the sign of a coefficient, then it must be equal to zero.

32
Objective Linear Ferro- magnets Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry 32 2nd Rank Tensor Properties & Symmetry The table from Nye shows the number of independent, non-zero coefficients allowed in a 2nd rank tensor according to the crystal symmetry class.

33
Objective Linear Ferro- magnets Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry 33 Effect of symmetry on stiffness matrix Following Reid, p.66 et seq.: Apply a 90° rotation about the crystal-z axis (axis 3), C ijkl = O im O jn O ko O lp C mnop : C = C

34
Objective Linear Ferro- magnets Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry 34 Effect of symmetry, 2 Using P = P, we can equate coefficients and find that: C 11 =C 22, C 13 =C 23, C 44 =C 35, C 16 =-C 26, C 14 =C 15 = C 24 = C 25 = C 34 = C 35 = C 36 = C 45 = C 46 = C 56 = 0.

35
Objective Linear Ferro- magnets Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry 35 Effect of symmetry, 3 Thus by repeated applications of the symmetry operators, one can demonstrate (for cubic crystal symmetry) that one can reduce the 81 coefficients down to only 3 independent quantities. These become two in the case of isotropy.

36
Objective Linear Ferro- magnets Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry 36 Cubic crystals: anisotropy factor If one applies the symmetry elements of the cubic system, it turns out that only three independent coefficients remain: C 11, C 12 and C 44, (similar set for compliance). From these three, a useful combination of the first two is C' = (C 11 - C 12 )/2 See Nye, Physical Properties of Crystals

37
Objective Linear Ferro- magnets Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry 37 Zeners anisotropy factor C' = (C 11 - C 12 )/2 turns out to be the stiffness associated with a shear in a direction on a plane. In certain martensitic transformations, this modulus can approach zero which corresponds to a structural instability. Zener proposed a measure of elastic anisotropy based on the ratio C 44 /C'. This turns out to be a useful criterion for identifying materials that are elastically anisotropic.

38
Objective Linear Ferro- magnets Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry 38 Rotated compliance (matrix) Given an orientation a ij, we transform the compliance tensor, using cubic point group symmetry, and find that:

39
Objective Linear Ferro- magnets Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry 39 Rotated compliance (matrix) This can be further simplified with the aid of the standard relations between the direction cosines, a ik a jk = 1 for i=j; a ik a jk = 0 for i j, (a ik a jk = ij ) to read as follows. By definition, the Youngs modulus in any direction is given by the reciprocal of the compliance, E = 1/S 11.

40
Objective Linear Ferro- magnets Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry 40 Anisotropy in cubic materials Thus the second term on the RHS is zero for directions and, for C 44 /C'>1, a maximum in directions (conversely a minimum for C 44 /C' is soft and is hard, with the exceptions of V and NaCl.

41
Objective Linear Ferro- magnets Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry 41 Stiffness coefficients, cubics [Courtney]

42
Objective Linear Ferro- magnets Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry 42 Anisotropy in terms of moduli Another way to write the above equation is to insert the values for the Young's modulus in the soft and hard directions, assuming that the are the most compliant direction(s). (Courtney uses,, and in place of my 1, 2, and 3. ) The advantage of this formula is that moduli in specific directions can be used directly.

43
Objective Linear Ferro- magnets Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry 43 Example Problem Should be E = 18.89 [Courtney]

44
Objective Linear Ferro- magnets Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry Alternate Vectorization 44 An alternate vectorization, discussed by Tomé on p287 of the Kocks et al. textbook, is to use the above set of eigentensors. For both stress and strain, one can matrix multiply each eigentensor into the stress/strain tensor in turn and obtain the coefficient of the corresponding stress/strain vector. Work conjugacy is still satisfied. The first two eigentensors represent shears in the {110} planes; the next three are simple shears on {110} systems, and the last (6 th ) is the hydrostatic component. The same vectorization can be used for plastic anisotropy, except in this case, the sixth, hydrostatic component is (generally) ignored.

45
Objective Linear Ferro- magnets Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry 45Summary We have covered the following topics: –Linear properties –Non-linear properties –Examples of properties –Tensors, vectors, scalars, tensor transformation law. –Elasticity, as example as of higher order property, also as example as how to apply (crystal) symmetry.

46
Objective Linear Ferro- magnets Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry 46 Supplemental Slides The following slides contain some useful material for those who are not familiar with all the detailed mathematical methods of matrices, transformation of axes, tensors etc.

47
Objective Linear Ferro- magnets Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry 47 Einstein Convention The Einstein Convention, or summation rule for suffixes looks like this: A i = B ij C j where i and j both are integer indexes whose range is {1,2,3}. So, to find eachi th component of A on the LHS, we sum up over the repeated index, j, on the RHS: A 1 = B 11 C 1 + B 12 C 2 + B 13 C 3 A 2 = B 21 C 1 + B 22 C 2 + B 23 C 3 A 3 = B 31 C 1 + B 32 C 2 + B 33 C 3

48
Objective Linear Ferro- magnets Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry 48 Matrix Multiplication Take each row of the LH matrix in turn and multiply it into each column of the RH matrix. In suffix notation, a ij = b ik c kj

49
Objective Linear Ferro- magnets Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry 49 Properties of Rotation Matrix The rotation matrix is an orthogonal matrix, meaning that any row is orthogonal to any other row (the dot products are zero). In physical terms, each row represents a unit vector that is the position of the corresponding (new) old axis in terms of the (old) new axes. The same applies to columns: in suffix notation - a ij a kj = ik, a ji a jk = ik ad+be+cf = 0 bc+ef+mn = 0

50
Objective Linear Ferro- magnets Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry 50 That the set of direction cosines are not independent is evident from the following construction: Thus, there are six relationships (i takes values from 1 to 3, and j takes values from 1 to 3) between the nine direction cosines, and therefore, as stated above, only three are independent, exactly as expected for a rotation. Another way to look at a rotation: combine an axis (described by a unit vector with two parameters) and a rotation angle (one more parameter, for a total of 3). Direction Cosines, contd.

51
Objective Linear Ferro- magnets Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry 51 Note that the direction cosines can be arranged into a 3x3 matrix,, and therefore the relation above is equivalent to the expression where T denotes the transpose of. This relationship identifies as an orthogonal matrix, which has the properties Orthogonal Matrices

52
Objective Linear Ferro- magnets Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry 52 When both coordinate systems are right-handed, det( )=+1 and is a proper orthogonal matrix. The orthogonality of also insures that, in addition to the relation above, the following holds: Combining these relations leads to the following inter- relationships between components of vectors in the two coordinate systems: Relationships

53
Objective Linear Ferro- magnets Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry 53 These relations are called the laws of transformation for the components of vectors. They are a consequence of, and equivalent to, the parallelogram law for addition of vectors. That such is the case is evident when one considers the scalar product expressed in two coordinate systems: Transformation Law

54
Objective Linear Ferro- magnets Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry 54 Thus, the transformation law as expressed preserves the lengths and the angles between vectors. Any function of the components of vectors which remains unchanged upon changing the coordinate system is called an invariant of the vectors from which the components are obtained. The derivations illustrate the fact that the scalar product is an invariant of and. Other examples of invariants include the vector product of two vectors and the triple scalar product of three vectors. The reader should note that the transformation law for vectors also applies to the components of points when they are referred to a common origin. Invariants

55
Objective Linear Ferro- magnets Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry 55 A rotation matrix,, is an orthogonal matrix, however, because each row is mutually orthogonal to the other two. Equally, each column is orthogonal to the other two, which is apparent from the fact that each row/column contains the direction cosines of the new/old axes in terms of the old/new axes and we are working with [mutually perpendicular] Cartesian axes. Orthogonality

56
Objective Linear Ferro- magnets Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry 56Anisotropy Anisotropy as a word simply means that something varies with direction. Anisotropy is from the Greek: aniso = different, varying; tropos = direction. Almost all crystalline materials are anisotropic; many materials are engineered to take advantage of their anisotropy (beer cans, turbine blades, microchips…) Older texts use trigonometric functions to describe anisotropy but tensors offer a general description with which it is much easier to perform calculations. For materials, what we know is that some properties are anisotropic. This means that several numbers, or coefficients, are needed to describe the property - one number is not sufficient. Elasticity is an important example of a property that, when examined in single crystals, is often highly anisotropic. In fact, the lower the crystal symmetry, the greater the anisotropy is likely to be. Nomenclature: in general, we need to use tensors to describe fields and properties. The simplest case of a tensor is a scalar which is all we need for isotropic properties. The next level of tensor is a vector, e.g. electric current.

57
Objective Linear Ferro- magnets Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry 57 Scalars, Vectors, Tensors Scalar:= quantity that requires only one number, e.g. density, mass, specific heat. Equivalent to a zero-rank tensor. Vector:= quantity that has direction as well as magnitude, e.g. velocity, current, magnetization; requires 3 numbers or coefficients (in 3D). Equivalent to a first-rank tensor. Tensor:= quantity that requires higher order descriptions but is the same, no matter what coordinate system is used to describe it, e.g. stress, strain, elastic modulus; requires 9 (or more, depending on rank) numbers or coefficients.

58
Objective Linear Ferro- magnets Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry 58 Vector field, response If we have a vector response, R, that we can write in component form, a vector field, F, that we can also write in component form, and a property, P, that we can write in matrix form (with nine coefficients) then the linearity of the property means that we can write the following ( R 0 = 0 ): R i = P ij F j A scalar (e.g. pressure) can be called a zero-rank tensor. A vector (e.g. electric current) is also known as a first-rank tensor.

59
Objective Linear Ferro- magnets Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry 59 Linear anisotropic property This means that each component of the response is linearly related to each component of the field and that the proportionality constant is the appropriate coefficient in the matrix. Example: R 1 = P 13 F 3, which says that the first component of the response is linearly related to the third field component through the property coefficient P 13. F3F3 R1R1 x1x1 x3x3

60
Objective Linear Ferro- magnets Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry 60 Example: electrical conductivity An example of such a linear anisotropic (second order tensor, discussed in later slides) property is the electrical conductivity of a material: Field: Electric Field, E Response: Current Density, J Property: Conductivity, J i = ij E j

61
Objective Linear Ferro- magnets Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry 61 Anisotropic electrical conductivity We can illustrate anisotropy with Nyes example of electrical conductivity, : Stimulus/ Field: E 1 0, E 2 =E 3 =0 Response: j 1 = 11 E 1, j 2 = 21 E 1, j 3 = 31 E 1, O

62
Objective Linear Ferro- magnets Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry 62 Changing the Coordinate System Many different choices are possible for the orthonormal base vectors and origin of the Cartesian coordinate system. A vector is an example of an entity which is independent of the choice of coordinate system. Its direction and magnitude must not change (and are, in fact, invariants), although its components will change with this choice. Why would we want to do something like this? For example, although the properties are conveniently expressed in a crystal reference frame, experiments often place the crystals in a non- symmetric position with respect to an experimental frame. Therefore we need some way of converting the coefficients of the property into the experimental frame. Changing the coordinate system is also known as axis transformation.

63
Objective Linear Ferro- magnets Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry 63 Tensor: definition, contd. In order for a quantity to qualify as a tensor it has to obey the axis transformation rule, as discussed in the previous slides. The transformation rule defines relationships between transformed and untransformed tensors of various ranks. Vector: V i = a ij V j 2 nd rank T ij = a ik a il T kl 3 rd rank T ijk = a il a im a kn T lmn 4 th rank T ijkl = a im a in a ko a lp T mnop This rule is a critical piece of information, which you must know how to use.

64
Objective Linear Ferro- magnets Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry Motivation for Axis Transformation One motivation for axis transformations is the need to solve problems where the specimen shape (and the stimulus direction) does not align with the crystal axes. Consider what happens when you apply a force parallel to the sides of this specimen … 64 [100] [110] The direction parallel to the long edge does not line up with any simple, low index crystal direction. Therefore we have to find a way to transform the properties that we know for the material into the frame of the problem (or vice versa). Image of Pt surface from www.cup.uni-muenchen.de/pc/wintterlin/IMGs/pt10p3.jpg Applied stress

65
Objective Linear Ferro- magnets Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry 65 Consider a new orthonormal system consisting of right- handed base vectors: These all have the same origin, o, associated with The vector v is clearly expressed equally well in either coordinate system: Note - same physical vector but different values of the components. We need to find a relationship between the two sets of components for the vector. New Axes

66
Objective Linear Ferro- magnets Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry 66 Anisotropy in Composites The same methods developed here for describing the anisotropy of single crystals can be applied to composites. Anisotropy is important in composites, not because of the intrinsic properties of the components but because of the arrangement of the components. As an example, consider (a) a uniaxial composite (e.g. tennis racket handle) and (b) a flat panel cross-ply composite (e.g. wing surface).

67
Objective Linear Ferro- magnets Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry 67 Fiber Symmetry x y z

68
Objective Linear Ferro- magnets Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry 68 Fiber Symmetry We will use the same matrix notation for stress, strain, stiffness and compliance as for single crystals. The compliance matrix, s, has 5 independent coefficients.

69
Objective Linear Ferro- magnets Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry 69Relationships For a uniaxial stress along the z (3) direction, This stress causes strain in the transverse plane: e 11 = e 22 = s 12 33. Therefore we can calculate Poissons ratio as: Similarly, stresses applied perpendicular to z give rise to different moduli and Poissons ratios.

70
Objective Linear Ferro- magnets Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry 70 Relationships, contd. Similarly the torsional modulus is related to shears involving the z axis, i.e. yz or xz shears: s 44 = s 55 = 1/G Shear in the x-y plane (1-2 plane) is related to the other compliance coefficients: s 66 = 2(s 11 -s 12 ) = 1/G xy

71
Objective Linear Ferro- magnets Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry 71 Plates: Orthotropic Symmetry Again, we use the same matrix notation for stress, strain, stiffness and compliance as for single crystals. The compliance matrix, s, has 9 independent coefficients. This corresponds to othorhombic sample symmetry: see the following slide with Table from Nyes book.

72
Objective Linear Ferro- magnets Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry 72 Plates: 0° and 90° plies If the composite is a laminate composite with fibers laid in at 0° and 90° in equal thicknesses then the symmetry is higher because the x and y directions are equivalent. The compliance matrix, s, has 6 independent coefficients. This corresponds to (tetragonal) 4mm sample symmetry: see the following slide with Table from Nyes book.

73
Objective Linear Ferro- magnets Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry 73 Effect of Symmetry on the Elasticity Tensors, S, C

74
Objective Linear Ferro- magnets Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry 74 General Anisotropic Properties Many different properties of crystals can be described as tensors. The rank of each tensor property depends, naturally, on the nature of the quantities related by the property.

75
Objective Linear Ferro- magnets Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry 75 Examples of Materials Properties as Tensors Table 1 shows a series of tensors that are of importance for material science. The tensors are grouped by rank, and are also labeled (in the last column) by E (equilibrium property) or T (transport property). The number following this letter indicates the maximum number of independent, nonzero elements in the tensor, taking into account symmetries imposed by thermodynamics. The Field and Response columns contain the following symbols: T = temperature difference, S = entropy change, E i = electric field components, H i = magnetic field components, ij = mechanical strain, D i = electric displacement, B i = magnetic induction, ij = mechanical stress, ij = change of the impermeability tensor, j i = electrical current density, j T = temperature gradient, h i = heat flux, j c = concentration gradient, m i = mass flux, a i = anti- symmetric part of resistivity tensor, s i = symmetric part of resistivity tensor, ij = change in the component ij of the resistivity tensor, l i = direction cosines of wave direction in crystal, G = gyration constant,

76
Objective Linear Ferro- magnets Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry 76

77
Objective Linear Ferro- magnets Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry 77 Courtesy of Prof. M. De Graef

78
Objective Linear Ferro- magnets Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry 78 Principal Effects Electrocaloric = pyroelectric Magnetocaloric = pyromagnetic Thermal expansion = piezocaloric Magnetoelectric and converse magnetoelectric Piezoelectric and converse piezoelectric Piezomagnetic and converse piezomagnetic Courtesy of Prof. M. De Graef

79
Objective Linear Ferro- magnets Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry 79 Principal Effects 1st rank cross effects 2nd rank cross effects 3rd rank cross effects Courtesy of Prof. M. De Graef

80
Objective Linear Ferro- magnets Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry 80 General crystal symmetry shown above. Courtesy of Prof. M. De Graef

81
Objective Linear Ferro- magnets Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry 81 Point group 4 Courtesy of Prof. M. De Graef

82
Objective Linear Ferro- magnets Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry 82 Point group m3m Note how many fewer independent coefficients there are! Note how the center of symmetry eliminates many of the properties, such as pyroelectricity Courtesy of Prof. M. De Graef

83
Objective Linear Ferro- magnets Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry 83Homogeneity Stimuli and responses of interest are, in general, not scalar quantities but tensors. Furthermore, some of the properties of interest, such as the plastic properties of a material, are far from linear at the scale of a polycrystal. Nonetheless, they can be treated as linear at a suitably local scale and then an averaging technique can be used to obtain the response of the polycrystal. The local or microscopic response is generally well understood but the validity of the averaging techniques is still controversial in many cases. Also, we will only discuss cases where a homogeneous response can be reasonably expected. There are many problems in which a non-homogeneous response to a homogeneous stimulus is of critical importance. Stress-corrosion cracking, for example, is a wildly non-linear, non-homogeneous response to an approximately uniform stimulus which depends on the mechanical and electro-chemical properties of the material.

Similar presentations

© 2017 SlidePlayer.com Inc.

All rights reserved.

Ads by Google